Superstructure-induced enhancement of solid-state triphenylacrylonitrile photochromism <i>via</i> a macrocycle-mediated blocking strategy.
Li, Meng-Hao; Hui, Hui; Wang, Yan; Yang, Ying-Wei; Chemical science 17 (2026) 5745–5757; doi:10.1039/d5sc08539j

data_1576898
_publ_section_title
;
 Superstructure-induced enhancement of solid-state triphenylacrylonitrile
 photochromism <i>via</i> a macrocycle-mediated blocking strategy.
;
_journal_issue                   11
_journal_name_full               'Chemical science'
_journal_page_first              5745
_journal_page_last               5757
_journal_paper_doi               10.1039/d5sc08539j
_journal_volume                  17
_journal_year                    2026
_chemical_formula_moiety         'C85 H72 N2 O8'
_chemical_formula_sum            'C85 H72 N2 O8'
_chemical_formula_weight         1249.44
_space_group_crystal_system      monoclinic
_space_group_IT_number           13
_space_group_name_Hall           '-P 2yac'
_space_group_name_H-M_alt        'P 1 2/n 1'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     iterative
_audit_creation_date             2025-09-24
_audit_creation_method
;
Olex2 1.5-alpha
(compiled 2025.07.13 svn.rb7424aed for OlexSys, GUI svn.r7317)
;
_audit_update_record
;
2025-09-24 deposited with the CCDC.	2026-01-22 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 102.146(6)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   15.5235(15)
_cell_length_b                   12.3965(10)
_cell_length_c                   20.4377(15)
_cell_measurement_reflns_used    9993
_cell_measurement_temperature    300.15
_cell_measurement_theta_max      26.91
_cell_measurement_theta_min      2.63
_cell_volume                     3844.9(6)
_computing_cell_refinement       'SAINT V8.40A (?, 2016)'
_computing_data_reduction        'SAINT V8.40A (?, 2016)'
_computing_molecular_graphics    'Olex2 1.5-alpha (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5-alpha (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'olex2.solve 1.5-alpha (Bourhis et al., 2015)'
_diffrn_ambient_temperature      300.15
_diffrn_measured_fraction_theta_full 0.987
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0684
_diffrn_reflns_av_unetI/netI     0.0327
_diffrn_reflns_Laue_measured_fraction_full 0.987
_diffrn_reflns_Laue_measured_fraction_max 0.987
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_number            81299
_diffrn_reflns_point_group_measured_fraction_full 0.987
_diffrn_reflns_point_group_measured_fraction_max 0.987
_diffrn_reflns_theta_full        24.999
_diffrn_reflns_theta_max         24.998
_diffrn_reflns_theta_min         2.740
_exptl_absorpt_coefficient_mu    0.069
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            'clear light colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    1.079
_exptl_crystal_description       block
_exptl_crystal_F_000             1320
_exptl_crystal_size_max          0.03
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.01
_platon_squeeze_details
;
TITL 1_pl             P 1 2/n 1    R = 0.26
CELL   15.5235   12.3965   20.4377     90.00    102.15     90.00
SPGR P2/n
C101 0.354 0.196 0.247 !       7.12 eA-3
C102 0.750 0.802 0.719 !       2.06 eA-3
C103 0.715 0.832 0.730 !       2.05 eA-3
C104 0.819 0.070 0.236 !       2.01 eA-3
C105 0.250 0.250 0.251 !       1.89 eA-3
C106 0.250 0.016 0.742 !       1.57 eA-3
C107 0.161 0.983 0.719 !       1.38 eA-3
C108 0.747 0.069 0.225 !       1.12 eA-3
C109 0.168 0.023 0.734 !       1.11 eA-3
C110 0.606 0.187 0.279 !       1.08 eA-3
Q111 0.710 0.024 0.314 !       0.98 eA-3
C112 0.407 0.841 0.769 !       0.91 eA-3
Q113 0.589 0.588 0.394 !       0.89 eA-3
Q114 0.403 0.358 0.079 !       0.84 eA-3
Q115 0.186 0.549 0.191 !       0.83 eA-3
Q116 0.061 0.591 0.190 !       0.83 eA-3
Q117 0.857 0.475 0.690 !       0.83 eA-3
Q118 0.143 0.525 0.310 !       0.83 eA-3
Q119 0.327 0.354 0.064 !       0.83 eA-3
C120 0.235 0.277 0.293 !       0.83 eA-3
Q121 0.987 0.654 0.156 !       0.81 eA-3
Q122 0.781 0.581 0.886 !       0.80 eA-3
Q123 0.255 0.373 0.439 !       0.79 eA-3
Q124 0.671 0.538 0.750 !       0.77 eA-3
Q125 0.704 0.502 0.641 !       0.76 eA-3
C126 0.922 0.077 0.264 !       0.76 eA-3
Q127 0.391 0.291 0.470 !       0.76 eA-3
Q128 0.873 0.443 0.799 !       0.75 eA-3
Q129 0.723 0.068 0.561 !       0.75 eA-3
Q130 0.824 1.005 0.202 !       0.74 eA-3
C131 0.902 0.118 0.227 !       0.73 eA-3
Q132 0.134 0.685 0.158 !       0.73 eA-3
Q133 0.341 0.469 0.207 !       0.72 eA-3
Q134 0.082 0.403 0.529 !       0.71 eA-3
Q135 0.731 0.469 0.718 !       0.71 eA-3
Q136 0.783 0.398 0.423 !       0.71 eA-3
Q137 0.730 0.126 0.271 !       0.69 eA-3
Q138 0.461 0.483 0.294 !       0.68 eA-3
C139 0.472 0.877 0.764 !       0.68 eA-3
Q140 0.114 0.391 0.655 !       0.67 eA-3
Q141 0.687 0.893 0.682 !       0.67 eA-3
Q142 0.629 0.155 0.204 !       0.67 eA-3
Q143 0.358 0.537 0.236 !       0.67 eA-3
Q144 0.831 0.026 0.859 !       0.66 eA-3
C145 0.449 0.199 0.278 !       0.66 eA-3
Q146 0.149 0.494 0.331 !       0.66 eA-3
Q147 0.818 0.395 0.394 !       0.66 eA-3
Q148 0.047 0.668 0.174 !       0.66 eA-3
C149 0.640 0.974 0.160 !       0.66 eA-3
Q150 0.657 0.372 0.501 !       0.66 eA-3
Q151 0.730 0.522 0.811 !       0.65 eA-3
Q152 0.982 0.484 0.174 !       0.65 eA-3
Q153 0.640 0.530 0.107 !       0.65 eA-3
Q154 0.808 0.892 0.686 !       0.65 eA-3
Q155 0.998 0.030 0.438 !       0.64 eA-3
Q156 0.237 0.235 0.640 !       0.63 eA-3
Q157 0.840 0.218 0.203 !       0.63 eA-3
Q158 0.746 0.069 0.309 !       0.63 eA-3
Q159 0.489 0.722 0.147 !       0.63 eA-3
Q160 0.276 0.316 0.277 !       0.62 eA-3
Q161 0.920 0.629 0.153 !       0.62 eA-3
Q162 0.750 0.406 0.749 !       0.62 eA-3
Q163 0.889 0.732 0.931 !       0.61 eA-3
Q164 0.142 0.920 0.428 !       0.61 eA-3
Q165 0.921 0.973 0.325 !       0.61 eA-3
Q166 0.781 0.412 0.359 !       0.61 eA-3
Q167 0.198 0.954 0.345 !       0.61 eA-3
Q168 0.405 0.996 0.124 !       0.60 eA-3
Q169 0.609 0.094 0.332 !       0.60 eA-3
Q170 0.718 0.596 0.404 !       0.60 eA-3
Q171 0.682 0.433 0.752 !       0.60 eA-3
Q172 0.250 0.422 0.751 !       0.59 eA-3
Q173 0.456 0.479 0.703 !       0.59 eA-3
Q174 0.341 0.622 0.329 !       0.59 eA-3
Q175 0.749 0.581 0.373 !       0.59 eA-3
Q176 0.344 0.933 0.881 !       0.59 eA-3
Q177 0.236 0.898 0.390 !       0.59 eA-3
Q178 0.768 0.478 0.377 !       0.59 eA-3
Q179 0.782 0.061 0.819 !       0.59 eA-3
Q180 0.312 0.928 0.064 !       0.59 eA-3
Q181 0.379 0.337 0.105 !       0.58 eA-3
Q182 0.674 0.566 0.145 !       0.58 eA-3
Q183 0.249 0.666 0.951 !       0.58 eA-3
Q184 0.063 0.877 0.692 !       0.57 eA-3
Q185 0.641 0.124 0.606 !       0.57 eA-3
Q186 0.577 0.798 0.543 !       0.57 eA-3
Q187 0.759 0.918 0.819 !       0.57 eA-3
Q188 0.517 0.597 0.379 !       0.57 eA-3
Q189 0.503 0.936 0.145 !       0.57 eA-3
Q190 0.500 0.985 0.679 !       0.57 eA-3
Q191 0.254 0.935 0.152 !       0.57 eA-3
Q192 0.203 0.456 0.657 !       0.56 eA-3
Q193 0.840 0.560 0.131 !       0.56 eA-3
Q194 0.669 0.875 0.158 !       0.56 eA-3
Q195 0.893 0.616 0.442 !       0.56 eA-3
Q196 0.136 0.316 0.013 !       0.56 eA-3
Q197 0.708 0.937 0.281 !       0.56 eA-3
Q198 0.591 0.029 0.278 !       0.56 eA-3
Q199 0.282 0.921 0.860 !       0.55 eA-3
;
_refine_diff_density_max         0.257
_refine_diff_density_min         -0.261
_refine_diff_density_rms         0.047
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.078
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     437
_refine_ls_number_reflns         6709
_refine_ls_number_restraints     30
_refine_ls_restrained_S_all      1.092
_refine_ls_R_factor_all          0.1153
_refine_ls_R_factor_gt           0.1004
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0320P)^2^+8.5000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1950
_refine_ls_wR_factor_ref         0.2042
_reflns_Friedel_coverage         0.000
_reflns_number_gt                5592
_reflns_number_total             6709
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d5sc08539j2.cif
_cod_data_source_block           1_pl_sq
_cod_database_code               1576898
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_max   0.999
_shelx_estimated_absorpt_t_min   0.998
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups
 At 1.5 times of:
  All C(H,H,H) groups
2. Uiso/Uaniso restraints and constraints
Uanis(C7) \\sim Ueq, Uanis(O2) \\sim Ueq, Uanis(C2) \\sim Ueq, Uanis(C8) \\sim
Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(C9) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
3. Others
 Fixed Sof: H8A(0.5) H8B(0.5)
4.a Secondary CH2 refined with riding coordinates:
 C8(H8A,H8B), C10(H10A,H10B), C19(H19A,H19B)
4.b Aromatic/amide H refined with riding coordinates:
 C2(H2), C5(H5), C12(H12), C15(H15), C24(H24), C25(H25), C27(H27), C28(H28),
 C33(H33), C34(H34), C35(H35), C36(H36), C37(H37), C39(H39), C40(H40), C41(H41),
  C42(H42), C43(H43)
4.c Idealised Me refined as rotating group:
 C7(H7A,H7B,H7C), C9(H9A,H9B,H9C), C17(H17A,H17B,H17C), C18(H18A,H18B,H18C)
;
_shelx_res_checksum              99971
_shelx_fab_checksum              65330
_platon_squeeze_void_probe_radius 1.20
_olex2_submission_special_instructions 'No special instructions were received'